# EROSION AND DEPOSITION MECHANISMS IN FUSION PLASMAS. A. Kirschner

Size: px
Start display at page:

## Transcription

2 II. EROSION MECHANISMS The erosion yield Y To characterize the strength of erosion the yield Y is defined as ratio of the averaged number of eroded particles and number of incoming projectiles. It is important to mention that not a single projectile is considered but a large amount of projectiles such that the erosion yield represents the erosion probability. The yield can be determined by the flux of eroded particles Γ ero divided by the flux of incoming projectiles Γ in : number of incoming projectiles Γ = (1a) in area time iii) Spike regime At high impact energies (kev MeV) and high projectile masses the densities of recoils of the collision cascade is increasing. Inside the spike region most atoms are moving, whereby collisions between simultaneously moving particles become important. Figure 1 illustrates these different regimes. The first two regimes can be described with the binary collision approximation (BCA), which will be discussed in chapter II.A.2. In the spike regime many-body processes have to be taken into account and the heat spike can lead to a local melting of the solid. However, under the conditions of wall materials in fusion experiments the spike regime is less important than the other two regimes. number of eroded atoms Γ = (1b) ero area time Γ Y = ero (1c) Γ in II.A. PHYSICAL SPUTTERING II.A.1. Basic features Within the process of physical sputtering, the momentum of incoming projectiles (energetic ions or neutrals) is transferred to surface atoms of the target material via nuclear collisions. If the transferred energy is large enough to overcome the surface binding energy (which is only known for a few materials, therefore it is common to use the heat of sublimation as an estimate), the surface atom can leave the solid and is physically sputtered. Although the first momentum transfer from projectile to target atoms is directed into the surface, subsequent collisions can lead to a momentum transfer which is directed out of the solid surface. Different regimes of collision can be distinguished mainly depending on the projectile energy and mass: i) Single collision regime After one single collision of the projectile with a target atom, the projectile hits a surface target atom. This process particularly occurs for light projectile ions with low impact energies. ii) Linear cascade regime Using medium projectile energies (larger than several 10 ev) a collision cascade is developing in the solid including also the generation of recoil atoms. However, collisions between two moving atoms are rare. single collision regime linear cascade regime spike regime Fig. 1. Collision regimes inside a solid induced by impact of a projectile atom. In general, physical sputtering occurs for all combinations of projectile and target materials. The sputtered species are mostly neutral atoms or small clusters of the target material. Due to the nature of physical sputtering there exists a threshold energy for projectile particles below which the sputtering yield is zero. A surface atom at least has to receive the surface binding energy to be sputtered from the solid. Besides the impact energy the sputtering yield also depends on the impact angle of projectiles. Also the combination of projectile and substrate material influences the sputter yield. This can be easily understood in terms of the maximum energy transfer factor γ for head-on collisions γ 4 M M 1 2 = (2) 2 (M1 + M 2 ) where M 1 and M 2 are the masses of projectile and target material respectively. The factor γ is maximal (= 1) for identical masses of projectile and substrate, M 1 = M 2. Physical sputtering does not significantly depend on the surface temperature but is dominated by the kinetics of collisions. The basics of physical sputtering of single-ion targets, covering theoretical aspects as well as experimental results, are described in 4. In the following the main dependencies of the sputtering yield are discussed in more detail.

3 Energy dependence of Y phys Below the threshold energy E th the sputter yield is zero. The threshold energy can be estimated for light projectile ions when only two collisions between projectile and solid atoms are involved as shown in Fig. 1, left part. In the extreme case of head-on collisions the projectile of impact energy E 0 has the energy (1 - γ) E 0 after reflection at the solid atom. The reflected projectile then can transfer a maximum energy of γ (1 - γ) E 0 to a surface atom of the solid. The sputtered atom finally has an energy of E sputt = γ (1 - γ) E 0 E B, where E B is the surface binding energy. From this, the threshold energy follows by setting E sputt = 0, thus: E th = E B γ (1 γ) (3) TABLE I. summarizes threshold energies for sputtering of beryllium, carbon (low-z) and tungsten (high-z) due to deuterium (D) and oxygen (O) as calculated with Eq. (3). As can be seen for sputtering caused by deuterium bombardment, the threshold energy for high-z materials is significantly larger than for low-z ones. In addition, the sputtering of high-z materials due to impurities such as oxygen starts at lower energies than the sputtering due to deuterium. However, Eq. (3) cannot be used universally for calculating threshold energies of physical sputtering. If the masses of projectile and target atoms are similar, wrong threshold energies are delivered (as shown in TABLE I. for sputtering of beryllium and carbon due to oxygen). This can be easily seen for the extreme case of M 1 = M 2 which gives γ = 1 and E th in Eq. (3) would be infinity. Though, with M 1 = M 2 one faces the situation of so-called self-sputtering, which is a very effective mechanism and cannot be explained with the simple two-collisions model. For the case of M 1 /M 2 > 0.2 a fit of experimental data 5 results in E 2/5 M 1 th = 8E B M (4) 2 For M 1 /M 2 < 0.2 Eq. (3) still is a good approximation of experimental data. The threshold energies according to Eq. (4) for the material combinations discussed so far with M 1 /M 2 > 0.2 are added in TABLE I. in brackets. TABLE I. Threshold energies (ev) for physical sputtering calculated acc. to Eq. (3) and Eq. (4) in brackets. D O Be (E B = 3.38 ev) 14 (15) 47 (34) C (E B = 7.42 ev) 46 ( ) 373 (67) W (E B = 8.8 ev) 214 ( ) 42 ( ) For impact energies above the threshold energy physical sputtering occurs with the sputter yield increasing monotonically until reaching a maximum value at a certain impact energy: more energy can be transferred to surface atoms, which increases the probability for sputtering. Further increase of the impact energy leads to continuous decrease of the sputter yield: the impinging projectiles and therefore also the collision cascades penetrate deeper into the solid and therefore less energy is transferred to surface atoms. Figure 2 shows as an example the energy dependence of physical sputtering of beryllium due to deuterium at normal incidence calculated with the TRIM 6 code. Sputtering Yield D on Be (normal incidence) Impact Energy (ev) Fig. 2. Calculated sputtering yield for D on Be: energy dependence. It is worth to mention that in a plasma, and therefore also in fusion experiments, the impact energy of ions hitting a surface is determined by the ion and electron temperature (T i and T e ), where in many cases E in ~ 3 Q T e +2 T i (5) with Q as the charge state of the projectile 7. The first part of Eq. (5) originates from the acceleration of the ions in the sheath potential and the second part reflects the Maxwell-distributed thermal velocity of the ions. Angular dependence of Y phys The angle of incidence α 0 of impinging projectiles is defined as angle between the velocity vector of the projectile and the surface normal vector. With this definition α 0 = 0 represents normal and α 0 = 90 grazing incidence. Figure 3 shows the calculated sputtering yield again for deuterium on beryllium but now with a fixed impact energy E 0 = 200 ev in dependence on the angle of incidence (data from TRIM calculations). Starting at normal incidence the sputter yield increases with increasing angle of incidence. With more grazing incidence of the projectiles more energy is deposited near the surface. After reaching a maximum yield (in the example of Fig. 3 at about 75 ) the sputtering yield strongly decreases. At theses shallow angles

4 reflection of projectiles becomes more important resulting in less energy available at the surface for sputtering. The described angular dependence of physical sputtering assumes smooth target surfaces. Unpolished surfaces normally exhibit a certain roughness. Sputtering Yield D on Be (E 0 = 200 ev) Angle of Incidence ( ) Fig. 3. Calculated (TRIM) sputtering yield for D on Be: angular dependence. Figure 4 demonstrates the effect of surface roughness on the sputter yield on the example of beryllium sputtering due to 300 ev deuterium ions 8. TRIM simulation assume smooth surface and deviate from measurements at a rough surface especially showing a more pronounced increase with nominal angle of incidence. At rough surfaces two processes have to be taken into account: First, the local angle of incidence differs from the nominal one. Dependent on the nominal angle of incidence one has to consider a distribution of local angles of incidence instead of one fixed angle. Taking e.g. a nominal angle of incidence of 0, leads to contributions of larger angles in the distribution of local angles of incidence. Thus, at a rough surface the sputter yield will be larger than at a smooth surface taking into account the angular dependence of Fig. 3. Sputtering Yield Angle of Incidence ( ) Fig. 4. Measured and calculated sputter yields of D on Be in dependence on the nominal angle of incidence for a rough surface 8. Similarly, at high nominal angles the sputter yield for rough surfaces will be smaller than for smooth ones especially the maximum yield for a rough surface will be smaller than for a smooth surface. Secondly, sputtered particles can be re-deposited at side walls of valleys on the rough surface. This effect decreases the sputtering yield. Obviously the importance of re-deposition increases with surface roughness and is less important at glancing nominal angles of incidence. Both effects, the distribution of local angles of incidence and re-deposition of sputtered particles, are included in the simulation of Fig. 4 for rough surfaces demonstrating a good agreement with the measured data. Energy and angular distribution of sputtered particles In many cases the energy distribution of sputtered particles can be described with a Thompson distribution: N(E sputt ) E sputt (6) 3 (E + E ) sputt B At E sputt = E B /2 the energy distribution has a maximum. At higher energies the probability for sputtered particles with the given energy decreases with 1/E 2. The maximal energy, which can be transferred to sputtered max particles equals Esputt = γ (1 γ) E0 E B and therefore has to be included in Eq. (6) as cut-off. Measurements of the energy distribution of sputtered particles agree fairly well with Eq. (6) for heavy-ion sputtering at normal incidence in the range of 1 kev 9, whereas deviations occur for light impact ions and/or non-normal incidence. The angular distribution of sputtered particles for normal incidence by medium and heavy ions can be approximated with a cosine distribution. This follows from the theory of cascade sputtering with the assumption of an isotropic collision cascade. Deviations to an overcosine distribution, which peaks towards the surface normal, arise for light-ion bombardment. This deviation tends to be stronger with low impact energies and/or metals with high surface binding energy 10. In practice surfaces are rough and data of angle distributions are rare, thus a cosine distribution is a good approximation. II.A.2. Calculating of physical sputtering yields Experimental data on physical sputtering yields are mainly obtained by means of ion beam irradiation were energetic ions are focused to a target. The sputter yield can then be determined by weight loss measuring of the target probe after bombardment. However, at low bombarding energies especially near the threshold energy of physical sputtering ion beam intensities become very low. Therefore measured data at low impact energies are rare and more uncertain. Modeling can help to close this gap.

5 To calculate the physical sputtering yield in dependence on the impact energy and angle fit formulae have been developed. Mostly the Bohdansky formula is used, which gives the yield for normal incidence in dependent on the impact energy 5. The overall accuracy of this formula is about a factor of 2 3. Meanwhile several improvements of this analytic formula have been provided. New attempts have been done for a unified representation of the physical sputtering yield in dependent on the impact energy 11. The dependence on the impact angle is described by the Yamamura formula 12. Again the accuracy is not better than a factor of 2. A more detailed approach to calculate sputtering yields is based on the modeling of the transport of the impinging projectile inside the solid. The TRIM 13 (TRansport of Ions in Matter) code and its derivative SDTrimSP 14 follow the projectiles through a randomized target in the binary collision approximation (BCA) and calculate the collision cascade including recoils. The critical parameter is the potential describing the interaction between projectile and target atoms. Various potentials are in use, such as the screened Coulomb potential for Kr-C 15, which is a good approximation for many projectile-solid atom combinations. Within the BCA the interaction between the projectile and the target atoms is treated by successive two-body interactions. This approximation breaks down at low impact energies (< ~10 ev) where many-body and quantum mechanical effects become important. More suitable for the situation of low impact energies (<10eV) are molecular dynamic (MD) simulations. Within MD calculations the motion is followed by the numerical solution of Newton s equations. For this, the many-body interaction potentials have to be known, which is a main constraint of MD calculations. Several methods exist to calculate these interaction potentials: the empirical approach ignores any quantum-mechanical effects or includes them by empirical methods. Semi-empirical potentials use the matrix representation from quantum mechanics, whereas the matrix elements themselves come from empirical formulae. Finally, ab-initio methods make use of full quantum-mechanical formulae. However, currently not all potentials necessary for plasma-wall interaction in fusion research are available especially there is still a lack of data where beryllium is involved. II.A.3. Sputtering of layered systems and mixed materials So far only physical sputtering of pure elements has been described. The mixing of different materials caused by deposition or implantation of impurities at the solid, leads to additional processes. One example is the sputtering of a carbon layer on top of a tungsten substrate due to deuterium ion impact, a situation which can occur at the tungsten baffles in ITER. Figure 5 shows the calculated (SDTrimSP) carbon sputtering yields in dependence on the deuterium ion impact energy for various thicknesses of a carbon layer on top of a tungsten substrate. As seen in Fig. 5, for thin carbon layers carbon sputtering becomes more effective compared with a pure carbon target. This can be explained by an increased reflection of incoming deuterium ions at the heavy tungsten substrate atoms compared to reflection on carbon atoms. Thus, more of the penetrating deuterium ions are reflected back to the surface where sputtering of carbon takes place. The enhanced sputtering occurs especially for thin layers and high projectiles impact energies. C Sputtering Yield C layer thickness 8 Å 80 Å (pure C) Electron Temperature [ev] Fig. 5. Physical sputtering yield of a carbon layer of varying thickness on top of a tungsten substrate (calculated with SDTrimSP). The impact energy E in of impinging D + ions is given as electron temperature T e (E in ~ 5T e ). In a more realistic situation the particles are implanted with a certain depth profile leading to different concentrations, which also depends on exposure time. However, the basic processes influencing the sputter yield are the same but the effects can be less pronounced than shown in Fig. 5. In nearly all cases of multi-element systems preferential sputtering of one of the components occurs, which can be reproduced with the TRIM and SDTrimSP code 16. Under multi-species conditions, further effects can occur like an oscillating of the partial sputtering yield in the case of heavy-ion bombardment of light targets (e.g. W ions on carbon target) 17. This effect is explained with fluence-dependent depth profiles of the implanted species. In addition to these collision-induced mechanisms, diffusion and segregation will influence the physical sputtering in mixed material systems. II.B. CHEMICAL EROSION Chemical erosion involves thermal projectiles (in contrast to energetic ones in the process of chemical sputtering) initiating chemical reactions with surface atoms. In contrast to physical sputtering chemical erosion

7 II.C. CHEMICAL SPUTTERING Chemical sputtering is defined as process where due to ion bombardment a chemical reaction occurs, which produces a particle weakly bound to the surface which then can be desorbed into the gas phase. The ion bombardment promotes the chemical reaction whereas the release of the particle itself is mainly thermally driven. Chemical sputtering depends on the kinetic energy and the chemical reactivity of the impinging species. The eroded species are molecules formed out of projectile and target atoms. In contrast to physical sputtering but similar to chemical erosion, chemical sputtering occurs only for certain combinations of projectile and target material. Again, in fusion research the interaction between hydrogen (and its isotopes) and carbon-based materials is most important, wherefore the following discussion will focus on this specific sputtering process. The threshold energy for chemical sputtering is significantly smaller than for physical sputtering and the chemical sputtering yield shows a clear dependence on the surface temperature of the substrate. As for chemical erosion also chemical sputtering leads to a wide range of sputtered hydrocarbon species. In addition to the surface temperature dependence the distribution of sputtered species also depends on the ion impact energy. Mechanism of chemical sputtering The energetic hydrogen ions penetrate into the solid and as long as they have enough energy the interaction with the solid atoms is determined by collision effects (leading to displacement of target atoms or physical sputtering). At the end of the projectile s trajectory, after thermalisation, chemical effects become important. This can be described by the model of chemical erosion as presented in the previous chapter a hydrocarbon complex can be formed with a yield Y therm. The hydrocarbon at the end of the ion range can then diffuse to the surface where it finally can leave the solid. However, in case of chemical sputtering the yield is enhanced compared to chemical erosion due to the effect of radiation damage of the penetrating energetic ion. The radiation damage in form of broken C-C bonds provides additional reaction sites for incoming H atoms and thus increases the probability of hydrocarbon formation. The yield for the enhanced thermal reaction can be written as Y damage therm = Y (1+ D Y ) (10) therm dam Here Y dam is the radiation damage yield, D a fit parameter to match experimental results. For Y dam one usually uses the physical sputtering yield but with a lower threshold energy. In addition to this damage-induced effect a process at the surface comes into play. It is observed experimentally that the hydrocarbon release under energetic ion bombardment starts at smaller surface temperatures than with thermal atom bombardment. This is explained by means of physical sputtering of weakly bound sp 3 CH x groups from the surface and described with a yield Y surf. The chemical sputtering yield can then be written as Y = Y (1+ D Y ) + Y (11) sputter chem therm dam The yield according to Eq. (11) depends on surface temperature, energy and flux of impinging hydrogen ions. By means of comparison with experimental data this has been used to formulate a semi-empirical formula to describe theses dependencies in detail 20. sputter Energy dependence of Y chem The chemical sputtering yield calculated according the formula in 20 is plotted in Fig. 8 in dependence on the impact energy for two surface temperatures and a hydrogen flux of m -2 s -1. At energies below ~ 2 ev only the thermal erosion process is active. At higher impact energies the yield is determined by the damageinduced (Y dam ) and the surface erosion (Y surf ) effect. The qualitative energy dependence is therefore similar to the one of physical sputtering (see Fig. 2). Chemical Sputtering Yield surf Impact Energy (ev) 400K 700K Fig. 8. Calculated chemical sputtering yield in dependence on hydrogen impact energy for surface temperatures of 400 and 700K (for Γ H = m -2 s -1 ). sputter Surface temperature dependence of Y chem Similar to chemical erosion also chemical sputtering shows a dependence on surface temperature. The common observation is a maximum of the sputtering yield about 900K. However, as will be discussed next, the surface temperature at which this maximum occurs also depends on the impinging hydrogen flux.

9 Ueda et al. Fig. 10. Total erosion yield of graphite due to Ar + bombardment in dependence on surface temperature 26. In Eq. (12) E RES is the activation energy for radiation enhanced sublimation ( ev) and Y 0 a pre-factor. RES is explained by the production of radiation defects (interstitials and vacancies) due to the energetic ions. The diffusion of the interstitials to the surface then competes with the annihilation with vacancies. Interstitials, which survive annihilation with vacancies, can arrive at the surface and desorb into the gas phase. However, up to now RES has not been observed clearly under tokamak particle impact conditions as e.g. shown in 27. This might be due to the high fluxes in combination with low energies. III. DEPOSITION MECHANISMS III.A. REFLECTION & DEPOSITION A projectile hitting a surface can be reflected (backscattered) from the surface with a certain probability which is expressed by the reflection coefficient R (0 R 1). Thus, the probability for a projectile of being deposited is 1-R. The reflected particles are in most cases neutrals. Similar to erosion yields reflection coefficients of atoms can be measured under well defined conditions in ion beam experiments. In case of molecular species other methods are in use as discussed later. Reflection data at fusion relevant low impact energies are rare. For calculation of reflection coefficients the same tools used for sputtering yield calculations can be applied (BCA based calculations such as TRIM, or MD simulations). III.A.1. Atomic species physical sputtering At first it is assumed that the projectile atoms interact with a smooth surface. Since reflection is governed by collisions between projectile and target atoms, the reflection coefficient depends on projectile and target masses (M 1, M 2 ) and impact energy and angle (E 0, α 0 ). Generally, the reflection coefficient increases with increasing mass ratio M 2 /M 1 the reflection of light projectiles at heavy substrate atoms is very effective. As example, the energy dependence of the reflection coefficient for carbon on carbon at an impact angle of 45 calculated with TRIM is shown in Fig. 11. At impact energies larger than ~200 ev the reflection coefficient decreases monotonically the projectiles penetrate deeper into the solid and the probability of implantation increases. The TRIM calculations show a steep decrease of reflection going to smaller impact energies. At E 0 < 20 ev the calculated reflection coefficient (Fig. 11) equals zero. However, as discussed in the previous chapter, the BCA method is not valid at such small impact energies below about 10 ev. MD calculations must be used under those conditions showing in contrast non-zero reflection coefficients even at impact energies less than 10 ev 28. Reflection Coefficient E-3 1E-4 C on C Impact Energy (ev) Fig. 11. Energy dependence of reflection coefficient R for carbon on carbon at impact angle of 45 (TRIM). The dependence of reflection on the impact angle is presented in Fig. 12 based on TRIM calculations for C on C at impact energy of 200 ev. With increasing angle of incidence the reflection probability increases: with more grazing incidence the projectile penetrates less deep into the solid which decreases the implantation probability. Reflection Coefficient C on C Angle of Incidence ( ) Fig. 12. Angle dependence of reflection coefficient R for carbon on carbon at impact energy of 200 ev (TRIM).

13 The surface temperature dependence of chemical sputtering yield corresponds well with the one described in chapter II. After a maximum yield at a certain temperature a significant decrease arises at higher temperatures. Maximum yield of about 4% occurs at a surface temperature of ~950K. IV.A.2. Methane injection experiments in TEXTOR Redeposition of chemically eroded hydrocarbons is an important issue for ITER, mainly due to tritium retention in such layers. In TEXTOR this has been investigated in detail by injecting 13 C marked methane CH 4 through test limiters of different shape (spherical or roof-like) and material (graphite, tungsten and molybdenum) 43, 44. The 13 C marked methane has been chosen to distinguish natural 12 C deposition caused by background plasma from the deposition caused by local injection. Figure 17 shows exemplarily the tungsten limiters (roof-like and spherical shape) after local 13 CH 4 injection demonstrating deposition near the injection hole. The broader dark region on the bottom part of the spherical limiter results from carbon 12 C deposition. Fig. 17. Tungsten test limiters after plasma exposure in TEXTOR with local methane 13 CH 4 injection. In all these experiments the local 13 C deposition efficiency (ratio of locally deposited 13 C on the test limiter surface and injected 13 C) was very small: for spherical limiters 0.3% on tungsten and 4% on graphite and for roof-like limiters 0.17% on molybdenum, 0.11% on tungsten and 0.17% on graphite. The substrate dependence of the 13 C deposition can be reproduced by SDTrimSP and is explained by a more effective erosion of thin carbon layers if the underlying substrate has a higher atom mass, see also Fig. 5. The larger deposition efficiency on spherical limiters can be explained with a flux dilution due to grazing incidence of the magnetic field at top of these limiters, leading to decreased erosion of deposited material. The described experiments have been modeled with the impurity transport code ERO 45. The low 13 C deposition efficiencies can be reproduced only if an enhanced erosion of redeposited carbon compared to graphite at plasma-wetted areas is assumed 46, 47. Using standard values for hydrocarbon sticking and re-erosion of redeposited carbon, the modeled 13 C redeposition efficiency is typically in the 50% range. A possible explanation for this enhanced erosion is an ion-induced desorption of loosely bound hydrocarbons that are freshly redeposited on the surface. This effect has direct influence on ITER since it provides a process for carbon transport at plasma-wetted areas triggered by successive re-deposition and re-erosion until finally layer formation (and tritium retention) takes place at plasma-shadowed regions. Experiments with varying surface roughness show an increase of 13 C deposition with roughness. Particles deposited inside the valleys of a rough surface are obviously more protected from the incident flux, which in the overall decreases the erosion of deposited 13 C. This is in agreement with the effect of surface roughness on physical sputtering as discussed in chapter II.A. IV.A.3. High-Z test limiter experiments in TEXTOR The sputtering of high-z materials has been investigated on test limiters by in-situ by spectroscopy. It is seen that the effective sputtering yield normalized to the impinging deuterium ion flux varies between 0.5 % at high edge density and 3% at low density 48. These yields cannot arise from deuterium sputtering alone but actually are dominated by carbon and oxygen impurity sputtering. Comparison with calculated sputtering yields lead to good agreement if also prompt redeposition of sputtered tungsten is taken into account. The erosion of tungsten from these limiters at elevated surface temperatures up to melting of W (3700K) does not show an enhanced yield compared to the expected physical sputtering 49. IV.B. ELM-INDUCED ENHANCED EROSION IN JET JET (Joint European Torus, located in Culham, UK) is presently the largest fusion research experiment in the world and therefore the most ITER-relevant device with respect to size and magnetic field configuration. The major plasma radius is 2.96 m and the minor radius of the D-shaped plasma is 2.1 m in vertical and 1.25 m in horizontal direction. As ITER, it is a divertor machine, in which the magnetic field lines are diverted by means of special coils into the divertor chamber. At the divertor plates the main plasma-wall interaction takes place. Details of the divertor concept can be found in 31. Main wall and divertor tiles of JET are made out of graphite. Deposition in the divertor of JET can be measured shot-resolved with Quartz Micro Balances (QMB) 40. One QMB is mounted in the inner divertor of JET (see Fig. 18.). With the magnetic configuration as indicated in Fig.18, deposition at this QMB represents erosion on tile #4, where the strike point (SP) is located. The right part of Fig.18 shows the carbon deposition on the QMB for high confinement discharges (H-mode) in dependent on ELM energy to the divertor ELMs are periodic energy bursts

### Chemical Erosion and Critical Issues for ITER

Chemical Erosion and Critical Issues for ITER J. Roth Max-Planck-Institut für Plasmaphysik, Garching Chemical Erosion Studies Erosion yields: Dependence on temperature, energy and flux Emitted hydrocarbons

### Chemical Sputtering of Carbon Materials due to Combined Bombardment by Ions and Atomic Hydrogen

Chemical Sputtering of Carbon Materials due to Combined Bombardment by Ions and Atomic Hydrogen W. Jacob, C. Hopf, and M. Schlüter Max-Planck-Institut für Plasmaphysik, EURATOM Association, Boltzmannstr.

### Modelling of Carbon Erosion and Deposition in the Divertor of JET

EFDA JET CP(01)02-64 A. Kirschner, V. Philipps, P. Wienhold, W. Fundamenski, G. Matthews, P. Coad, M. Stamp, D. Coster, D. Elder, P. Stangeby and JET EFDA Contributors Modelling of Carbon Erosion and Deposition

### Molecular Dynamics Study of Plasma Surface Interactions for Mixed Materials

J. Plasma Fusion Res. SERIES, Vol. 9 () Molecular Dynamics Study of Plasma Surface Interactions for Mixed Materials Kaoru OHYA, Naohide MOHARA, Kensuke INAI, Atsushi ITO, Hiroaki NAKAMURA, Yoshio UEDA

### Surface processes during thin-film growth

Plasma Sources Sci. Technol. 9 (2000) 455 467. Printed in the UK PII: S0963-0252(00)15187-4 Surface processes during thin-film growth Achim von Keudell Max-Planck-Institut für Plasmaphysik, Boltzmannstrasse

### Estimation of the contribution of gaps to tritium retention in the divertor of ITER

Estimation of contribution of gaps to tritium retention in the divertor of ITER 1 Estimation of the contribution of gaps to tritium retention in the divertor of ITER 1. Introduction D. Matveev 1,2, A.

### Implantation Energy Dependence on Deuterium Retention Behaviors for the Carbon Implanted Tungsten

J. Plasma Fusion Res. SERIES, Vol. 10 (2013) Implantation Energy Dependence on Deuterium Retention Behaviors for the Carbon Implanted Tungsten Yasuhisa Oya 1) *, Makoto Kobayashi 1), Naoaki Yoshida 2),

### In-vessel Tritium Inventory in ITER Evaluated by Deuterium Retention of Carbon Dust

FT/P1-19 In-vessel Tritium Inventory in ITER Evaluated by Deuterium Retention of Carbon Dust T. Hino 1), H. Yoshida 1), M. Akiba 2), S. Suzuki 2), Y. Hirohata 1) and Y. Yamauchi 1) 1) Laboratory of Plasma

### 1 EX/P4-8. Hydrogen Concentration of Co-deposited Carbon Films Produced in the Vicinity of Local Island Divertor in Large Helical Device

1 EX/P4-8 Hydrogen Concentration of Co-deposited Carbon Films Produced in the Vicinity of Local Island Divertor in Large Helical Device T. Hino 1,2), T. Hirata 1), N. Ashikawa 2), S. Masuzaki 2), Y. Yamauchi

### Hydrocarbon transport in the MkIIa divertor of JET

INSTITUTE OF PHYSICS PUBLISHING Plasma Phys. Control. Fusion 45 (23) 39 319 PLASMA PHYSICS AND CONTROLLED FUSION PII: S741-3335(3)37188-X Hydrocarbon transport in the MkIIa divertor of JET A Kirschner

### Thomas Schwarz-Selinger. Max-Planck-Institut for Plasmaphysics, Garching Material Science Division Reactive Plasma Processes

Max-Planck-Institut für Plasmaphysik Thomas Schwarz-Selinger Max-Planck-Institut for Plasmaphysics, Garching Material Science Division Reactive Plasma Processes personal research interests / latest work

### Tokamak Divertor System Concept and the Design for ITER. Chris Stoafer April 14, 2011

Tokamak Divertor System Concept and the Design for ITER Chris Stoafer April 14, 2011 Presentation Overview Divertor concept and purpose Divertor physics General design considerations Overview of ITER divertor

### Multiscale modelling of D trapping in W

CMS Multiscale modelling of D trapping in W Kalle Heinola, Tommy Ahlgren and Kai Nordlund Department of Physics and Helsinki Institute of Physics University of Helsinki, Finland Contents Background Plasma-wall

### Max-Planck-Institut für Plasmaphysik, EURATOM Association POB 1533, D Garching, Germany

DEPTH PROFILE REONSTRUTION FROM RUTHERFORD BAKSATTERING DATA U. V. TOUSSAINT, K. KRIEGER, R. FISHER, V. DOSE Max-Planck-Institut für Plasmaphysik, EURATOM Association POB 1533, D-8574 Garching, Germany

### Helium effects on Tungsten surface morphology and Deuterium retention

1 Helium effects on Tungsten surface morphology and Deuterium retention Y. Ueda, H.Y. Peng, H. T. Lee (Osaka University) N. Ohno, S. Kajita (Nagoya University) N. Yoshida (Kyushu University) R. Doerner

### Comparison of tungsten fuzz growth in Alcator C-Mod and linear plasma devices

Comparison of tungsten fuzz growth in Alcator C-Mod and linear plasma devices G.M. Wright 1, D. Brunner 1, M.J. Baldwin 2, K. Bystrov 3, R. Doerner 2, B. LaBombard 1, B. Lipschultz 1, G. de Temmerman 3,

### 31704 Dynamic Monte Carlo modeling of hydrogen isotope. reactive-diffusive transport in porous graphite

31704 Dynamic Monte Carlo modeling of hydrogen isotope reactive-diffusive transport in porous graphite * R. Schneider a, A. Rai a, A. Mutzke a, M. Warrier b,e. Salonen c, K. Nordlund d a Max-Planck-Institut

### Progress Report on Chamber Dynamics and Clearing

Progress Report on Chamber Dynamics and Clearing Farrokh Najmabadi, Rene Raffray, Mark S. Tillack, John Pulsifer, Zoran Dragovlovic (UCSD) Ahmed Hassanein (ANL) Laser-IFE Program Workshop May31-June 1,

### Sputtering by Particle Bombardment

Rainer Behrisch, Wolfgang Eckstein (Eds.) Sputtering by Particle Bombardment Experiments and Computer Calculations from Threshold to MeV Energies With 201 Figures e1 Springer Contents Introduction and

### Chapter 6. Summary and Conclusions

Chapter 6 Summary and Conclusions Plasma deposited amorphous hydrogenated carbon films (a-c:h) still attract a lot of interest due to their extraordinary properties. Depending on the deposition conditions

### Computer-Simulation Studies of Plasma- Surface Interactions

Computer-Simulation Studies of Plasma- Surface Interactions T. Ono ) Collabrators: T. Kawamura 2), T. Muramoto ), S.T. Nakagawa ), T. Kenmotsu 3) ) Okayama Univ. of Science, - Ridai-cho, Okayama 700-0005,

### Modeling Plasma Interactions with ITER Wall Materials: Erosion, Transport, Redeposition, Reerosion and Material Mixing, and Tritium Retention

Modeling Plasma Interactions with ITER Wall Materials: Erosion, Transport, Redeposition, Reerosion and Material Mixing, and Tritium Retention Kaoru Ohya Institute of Technology and Science, The University

### ITER A/M/PMI Data Requirements and Management Strategy

ITER A/M/PMI Data Requirements and Management Strategy Steven Lisgo, R. Barnsley, D. Campbell, A. Kukushkin, M. Hosokawa, R. A. Pitts, M. Shimada, J. Snipes, A. Winter ITER Organisation with contributions

### Atomistic simulations of plasma-material interactions in fusion reactors

UNIVERSITY OF HELSINKI REPORT SERIES IN PHYSICS HU-P-D257 Atomistic simulations of plasma-material interactions in fusion reactors Elnaz Safi Division of Materials Physics Department of Physics Faculty

### Comparison of tungsten fuzz growth in Alcator C-Mod and linear plasma devices!

Comparison of tungsten fuzz growth in Alcator C-Mod and linear plasma devices G.M. Wright 1, D. Brunner 1, M.J. Baldwin 2, K. Bystrov 3, R. Doerner 2, B. LaBombard 1, B. Lipschultz 1, G. de Temmerman 3,

### Molecular Dynamics Simulation of Chemical Sputtering of Hydrogen Atom on Layer Structured Graphite

1 TH/7-1 Molecular Dynamics Simulation of Chemical Sputtering of Hydrogen Atom on Layer Structured Graphite A. Ito 1,2), Y. Wang 1), S. Irle 1), K. Morokuma 3), and H. Nakamura 2) 1) Nagoya University,

### Carbon Deposition and Deuterium Inventory in ASDEX Upgrade

1 IAEA-CN-116 / EX / 5-24 Carbon Deposition and Deuterium Inventory in ASDEX Upgrade M. Mayer 1, V. Rohde 1, J. Likonen 2, E. Vainonen-Ahlgren 2, J. Chen 1, X. Gong 1, K. Krieger 1, ASDEX Upgrade Team

### Chapter IX: Nuclear fusion

Chapter IX: Nuclear fusion 1 Summary 1. General remarks 2. Basic processes 3. Characteristics of fusion 4. Solar fusion 5. Controlled fusion 2 General remarks (1) Maximum of binding energy per nucleon

### Materials for Future Fusion Reactors under Severe Stationary and Transient Thermal Loads

Mitglied der Helmholtz-Gemeinschaft Materials for Future Fusion Reactors under Severe Stationary and Transient Thermal Loads J. Linke, J. Du, N. Lemahieu, Th. Loewenhoff, G. Pintsuk, B. Spilker, T. Weber,

### Comparisons of DFT-MD, TB- MD and classical MD calculations of radiation damage and plasmawallinteractions

CMS Comparisons of DFT-MD, TB- MD and classical MD calculations of radiation damage and plasmawallinteractions Kai Nordlund Department of Physics and Helsinki Institute of Physics University of Helsinki,

### Modeling and analysis of surface roughness effects on sputtering, reflection and sputtered particle transport *

278 Journai of Nuclear Materials 176 & 177 (1990) 278-282 North-Holland Modeling and analysis of surface roughness effects on sputtering, reflection and sputtered particle transport * J.N. Brooks Argonne

### PISCES W fuzz experiments: A summary of work up to now.

FNST/PFC/MASCO meeting, UCLA Aug. 2-6, 2010 W fuzz experiments: A summary of work up to now. M.J. Baldwin, R.P. Doerner, D. Nishijima University of California, San Diego, USA Why do we care about fuzz?

### Can we tend the fire?

Can we tend the fire? Three lectures course on plasma surface interaction and edge physics I Introduction: WHAT happens in a fusion plasma near the walls Detlev Reiter Forschungszentrum Jülich GmbH, Institut

### Neutral beam plasma heating

Seminar I b 1 st year, 2 nd cycle program Neutral beam plasma heating Author: Gabrijela Ikovic Advisor: prof.dr. Tomaž Gyergyek Ljubljana, May 2014 Abstract For plasma to be ignited, external heating is

### Isotope Exchange in High Heat-flux Components of the JET Tritium Neutral Beam Injector

JET CP(98)39 Isotope Exchange in High Heat-flux Components of the JET Neutral Beam Injector D Ciric, H P L de Esch, H-D Falter, T T C Jones, L Svensson. JET Joint Undertaking, Abingdon, Oxfordshire, OX14

### Fundamental science and synergy of multi-species surface interactions in high-plasma--flux environments

Fundamental science and synergy of multi-species surface interactions in high-plasma--flux environments Our thanks to John Hogan Managed by UT-Battelle for the Department of Energy ReNew PMI, UCLA, March

### Deposition and re-erosion studies by means of local impurity injection in TEXTOR

Deposition and re-erosion studies by means of local impurity injection in TEXTOR A. Kirschner a*, A. Kreter a, P. Wienhold a, S. Brezinsek a, J.W. Coenen a, H.G. Esser a, A. Pospieszczyk a, Ch. Schulz

### Deuterium and Hydrogen Retention Properties of the JT-60 and JT-60U Divertor Tiles

Deuterium and Hydrogen Retention Properties of the JT-60 and JT-60U Divertor Tiles Y. Hirohata 1), T. Tanabe 2), Y. Oya 3), K. Shibahara 4), M. Oyaidzu 5), T. Arai 6), K. Masaki 6), Y. Gotoh 6), K. Okuno

### PHYSICAL VAPOR DEPOSITION OF THIN FILMS

PHYSICAL VAPOR DEPOSITION OF THIN FILMS JOHN E. MAHAN Colorado State University A Wiley-Interscience Publication JOHN WILEY & SONS, INC. New York Chichester Weinheim Brisbane Singapore Toronto CONTENTS

### Plasma Wall Interactions in Tokamak

Plasma Wall Interactions in Tokamak Dr. C Grisolia, Association Euratom/CEA sur la fusion, CEA/Cadarache Outline 1. Conditions for Fusion in Tokamaks 2. Consequences of plasma operation on in vessel materials:

### Modelling of prompt deposition of tungsten under fusion relevant conditions

EUROFUSION WPPFC-CP(16) 1532 A Kirschner et al. Modelling of prompt deposition of tungsten under fusion relevant conditions Preprint of Paper to be submitted for publication in Proceedings of 26th IAEA

### Chapter V: Interactions of neutrons with matter

Chapter V: Interactions of neutrons with matter 1 Content of the chapter Introduction Interaction processes Interaction cross sections Moderation and neutrons path For more details see «Physique des Réacteurs

### Depth profiles of helium and hydrogen in tungsten nano-tendril surface morphology using Elastic Recoil Detection

PSFC/JA-12-82 Depth profiles of helium and hydrogen in tungsten nano-tendril surface morphology using Elastic Recoil Detection K.B. Woller, D.G. Whyte, G.M. Wright, R.P. Doerner*, G. de Temmerman** * Center

### The Spherical Tokamak as a Compact Fusion Reactor Concept

The Spherical Tokamak as a Compact Fusion Reactor Concept R. Kaita Princeton Plasma Physics Laboratory ENN Symposium on Compact Fusion Technologies April 19 20, 2018 *This work supported by US DOE Contract

### The role of PMI in MFE/IFE common research

The role of PMI in MFE/IFE common research Presented by Doerner for the Team and TITAN 1-1 Participants In 2006, Jupiter II recognized that PMI was a bridge issue between MFE and IFE R&D Both MFE and IFE

### Neutron Sources Fall, 2017 Kyoung-Jae Chung Department of Nuclear Engineering Seoul National University

Neutron Sources Fall, 2017 Kyoung-Jae Chung Department of Nuclear Engineering Seoul National University Neutrons: discovery In 1920, Rutherford postulated that there were neutral, massive particles in

### Effect of ExB Driven Transport on the Deposition of Carbon in the Outer Divertor of. ASDEX Upgrade

Association Euratom-Tekes ASDEX Upgrade Effect of ExB Driven Transport on the Deposition of Carbon in the Outer Divertor of ASDEX Upgrade L. Aho-Mantila 1,2, M. Wischmeier 3, K. Krieger 3, V. Rohde 3,

### Influence of Amorphous Carbon Deposition on the Probability for Recombination of Neutral Oxygen Atoms on Aluminium Surfaces

Influence of Amorphous Carbon Deposition on the Probability for Recombination of Neutral Oxygen Atoms on Aluminium Surfaces A. Drenik, A. Vesel Center of Excellence for Polymer Materials and Technologies

### DIVIMP simulation of W transport in the SOL of JET H-mode plasmas

DIVIMP simulation of W transport in the SOL of JET H-mode plasmas A. Järvinen a, C. Giroud b, M. Groth a, K. Krieger c, D. Moulton d, S. Wiesen e, S. Brezinsek e and JET- EFDA contributors¹ JET-EFDA, Culham

### Modelling of JT-60U Detached Divertor Plasma using SONIC code

J. Plasma Fusion Res. SERIES, Vol. 9 (2010) Modelling of JT-60U Detached Divertor Plasma using SONIC code Kazuo HOSHINO, Katsuhiro SHIMIZU, Tomonori TAKIZUKA, Nobuyuki ASAKURA and Tomohide NAKANO Japan

### EU Plasma-Wall Interactions Task Force

Recent results on material migration and fuel retention in JET V. Philipps and JET TFE co-workers* Overview on present results on erosion, deposition and fuel retention in last JET campaign (2001-2004,C5-C15)

### Introduction to Fusion Physics

Introduction to Fusion Physics Hartmut Zohm Max-Planck-Institut für Plasmaphysik 85748 Garching DPG Advanced Physics School The Physics of ITER Bad Honnef, 22.09.2014 Energy from nuclear fusion Reduction

### A Project for High Fluence 14 MeV Neutron Source

A Project for High Fluence 14 MeV Neutron Source Mario Pillon 1, Maurizio Angelone 1, Aldo Pizzuto 1, Antonino Pietropaolo 1 1 Associazione ENEA-EURATOM Sulla Fusione, ENEA C.R. Frascati, via E. Fermi,

### Interactions between ion thruster plumes and vessel walls

Interactions between ion thruster plumes and vessel walls IEPC-2013-xxx Presented at the 33 rd International Electric Propulsion Conference, The George Washington University, Washington, D.C., USA J. Duras,

### NJCTL.org 2015 AP Physics 2 Nuclear Physics

AP Physics 2 Questions 1. What particles make up the nucleus? What is the general term for them? What are those particles composed of? 2. What is the definition of the atomic number? What is its symbol?

13th International Workshop on Plasma-Facing Materials and Components for Fusion Applications / 1st International Conference on Fusion Energy Materials Science Comparison of deuterium retention for ion-irradiated

### AMS MEASUREMENTS OF DEUTERIUM CAPTURED IN TUNGSTEN LAYERS DEPOSITED BY MAGNETRON SPUTTERING

Romanian Reports in Physics, Vol. 65, No. 4, P. 1258 1264, 2013 AMS MEASUREMENTS OF DEUTERIUM CAPTURED IN TUNGSTEN LAYERS DEPOSITED BY MAGNETRON SPUTTERING A.R. PETRE 1,3, T. ACSENTE 2, M. ENACHESCU 1,

### Ion beam analysis methods in the studies of plasma facing materials in controlled fusion devices

Vacuum 70 (2003) 423 428 Ion beam analysis methods in the studies of plasma facing materials in controlled fusion devices M. Rubel a, *, P. Wienhold b, D. Hildebrandt c a Alfv!en Laboratory, Royal Institute

### Experience with Moving from Dpa to Changes in Materials Properties

Experience with Moving from Dpa to Changes in Materials Properties Meimei Li, Argonne National Laboratory N. V. Mokhov, Fermilab 46 th ICFA Advanced Beam Dynamics Workshop Sept. 27 Oct. 1, 2010 Morschach,

### Atomic physics in fusion development

Atomic physics in fusion development The next step in fusion development imposes new requirements on atomic physics research by R.K. Janev In establishing the scientific and technological base of fusion

### TMT4320 Nanomaterials November 10 th, Thin films by physical/chemical methods (From chapter 24 and 25)

1 TMT4320 Nanomaterials November 10 th, 2015 Thin films by physical/chemical methods (From chapter 24 and 25) 2 Thin films by physical/chemical methods Vapor-phase growth (compared to liquid-phase growth)

### Report A+M/PSI Data Centre NRC Kurchatov Institute

Report A+M/PSI Data Centre NRC Kurchatov Institute Yu.V.Martynenko 21st Meeting of the Atomic and Molecular Data Centers and ALADDIN Network Vienna, 07-09 September 2011 The main activities on A+M/PSI

### ETCHING Chapter 10. Mask. Photoresist

ETCHING Chapter 10 Mask Light Deposited Substrate Photoresist Etch mask deposition Photoresist application Exposure Development Etching Resist removal Etching of thin films and sometimes the silicon substrate

### R. Clark, D. Humbert, K. Sheikh Nuclear Data Section

Calculation of Atomic Data for Plasma Modeling: Introduction and Atomic Structure Part 1 R. Clark, D. Humbert, K. Sheikh Nuclear Data Section Overview Plasmas in fusion research Data needs for plasma modeling

### 6.5 Optical-Coating-Deposition Technologies

92 Chapter 6 6.5 Optical-Coating-Deposition Technologies The coating process takes place in an evaporation chamber with a fully controlled system for the specified requirements. Typical systems are depicted

### Effect of Spiral Microwave Antenna Configuration on the Production of Nano-crystalline Film by Chemical Sputtering in ECR Plasma

THE HARRIS SCIENCE REVIEW OF DOSHISHA UNIVERSITY, VOL. 56, No. 1 April 2015 Effect of Spiral Microwave Antenna Configuration on the Production of Nano-crystalline Film by Chemical Sputtering in ECR Plasma

### Introduction to Thin Film Processing

Introduction to Thin Film Processing Deposition Methods Many diverse techniques available Typically based on three different methods for providing a flux of atomic or molecular material Evaporation Sputtering

### Estimating the plasma flow in a recombining plasma from

Paper P3-38 Estimating the plasma flow in a recombining plasma from the H α emission U. Wenzel a, M. Goto b a Max-Planck-Institut für Plasmaphysik (IPP) b National Institute for Fusion Science, Toki 509-5292,

Radiative type-iii ELMy H-mode in all-tungsten ASDEX Upgrade J. Rapp 1, A. Kallenbach 2, R. Neu 2, T. Eich 2, R. Fischer 2, A. Herrmann 2, S. Potzel 2, G.J. van Rooij 3, J.J. Zielinski 3 and ASDEX Upgrade

### Molecular Dynamics Simulation of Hydrocarbon Reflection and Dissociation Coefficients from Fusion-Relevant Carbon Surfaces

Physica Scripta. Vol. T111, 145 151, 2004 Molecular Dynamics Simulation of Hydrocarbon Reflection and Dissociation Coefficients from Fusion-Relevant Carbon Surfaces D. A. Alman and D. N. Ruzic Department

### Applicability of Laser-Induced Desorption Quadruple Mass Spectrometry (LID-QMS) for the Determination of Local Deuterium Retention

Applicability of Laser-Induced Desorption Quadruple Mass Spectrometry (LID-QMS) for the Determination of Local Deuterium Retention Reinier Zoomers June 2013 Supervisors: Dr. Pedro Zeijlmans van Emmichoven

### Etching Issues - Anisotropy. Dry Etching. Dry Etching Overview. Etching Issues - Selectivity

Etching Issues - Anisotropy Dry Etching Dr. Bruce K. Gale Fundamentals of Micromachining BIOEN 6421 EL EN 5221 and 6221 ME EN 5960 and 6960 Isotropic etchants etch at the same rate in every direction mask

### Cesium Dynamics and H - Density in the Extended Boundary Layer of Negative Hydrogen Ion Sources for Fusion

Cesium Dynamics and H - Density in the Extended Boundary Layer of Negative Hydrogen Ion Sources for Fusion C. Wimmer a, U. Fantz a,b and the NNBI-Team a a Max-Planck-Institut für Plasmaphysik, EURATOM

### Atomic and Nuclear Physics. Topic 7.3 Nuclear Reactions

Atomic and Nuclear Physics Topic 7.3 Nuclear Reactions Nuclear Reactions Rutherford conducted experiments bombarding nitrogen gas with alpha particles from bismuth-214. He discovered that fast-moving particles

### Computer simulation of multi-elemental fusion reactor materials

UNIVERSITY OF HELSINKI REPORT SERIES IN PHYSICS HU-P-D186 Computer simulation of multi-elemental fusion reactor materials Katharina Vörtler Division of Materials Physics Department of Physics Faculty of

### is the minimum stopping potential for which the current between the plates reduces to zero.

Module 1 :Quantum Mechanics Chapter 2 : Introduction to Quantum ideas Introduction to Quantum ideas We will now consider some experiments and their implications, which introduce us to quantum ideas. The

### Dynamic Monte-Carlo modeling of hydrogen isotope reactive diffusive transport in porous graphite

Journal of Nuclear Materials 367 37 (27) 238 242 www.elsevier.com/locate/jnucmat Dynamic Monte-Carlo modeling of hydrogen isotope reactive diffusive transport in porous graphite R. Schneider a, *, A. Rai

### Plasma interactions with Be surfaces

Plasma interactions with Be surfaces R. P. Doerner and D. Nishijima for members of the Team Center for Energy Research, University of California San Diego, USA Work performed as part of: Plasma-Surface

### Hydrogenic retention of high-z refractory metals exposed to ITER divertor relevant plasma conditions

1 Hydrogenic retention of high-z refractory metals exposed to ITER divertor relevant plasma conditions G.M. Wright 1), E. Alves 2), L.C. Alves 2), N.P. Barradas 2), M. Mayer 3), G.J. van Rooij 1), R.S.

### Sputtering Yield of Noble Gas Irradiation onto Tungsten Surface

J. Adv. Simulat. Sci. Eng. Vol. 3, No. 2, 165 172. c 2016 Japan Society for Simulation Technology Sputtering Yield of Noble Gas Irradiation onto Tungsten Surface Hiroaki Nakamura 1,2,*, Seiki Saito 3,

### Radiation damage I. Steve Fitzgerald.

Radiation damage I Steve Fitzgerald http://defects.materials.ox.ac.uk/ Firstly an apology Radiation damage is a vast area of research I cannot hope to cover much in any detail I will try and introduce

### Lecture 31 Chapter 22, Sections 3-5 Nuclear Reactions. Nuclear Decay Kinetics Fission Reactions Fusion Reactions

Lecture Chapter, Sections -5 Nuclear Reactions Nuclear Decay Kinetics Fission Reactions Fusion Reactions Gamma Radiation Electromagnetic photons of very high energy Very penetrating can pass through the

### The New Sorgentina Fusion Source Project

The New Sorgentina Fusion Source Project P. Agostini, P. Console Camprini, D. Bernardi, M. Pillon, M. Frisoni, M. Angelone, A. Pietropaolo, P. Batistoni, A. Pizzuto ENEA Agenzia Nazionale per le Nuove

### CHAPTER 2 RADIATION INTERACTIONS WITH MATTER HDR 112 RADIATION BIOLOGY AND RADIATION PROTECTION MR KAMARUL AMIN BIN ABDULLAH

HDR 112 RADIATION BIOLOGY AND RADIATION PROTECTION CHAPTER 2 RADIATION INTERACTIONS WITH MATTER PREPARED BY: MR KAMARUL AMIN BIN ABDULLAH SCHOOL OF MEDICAL IMAGING FACULTY OF HEALTH SCIENCE Interactions

### Erosion/redeposition analysis of CMOD Molybdenum divertor and NSTX Liquid Lithium Divertor

Erosion/redeposition analysis of CMOD Molybdenum divertor and NSTX Liquid Lithium Divertor J.N. Brooks, J.P. Allain Purdue University PFC Meeting MIT, July 8-10, 2009 CMOD Mo tile divertor erosion/redeposition

### Interaction of ion beams with matter

Interaction of ion beams with matter Introduction Nuclear and electronic energy loss Radiation damage process Displacements by nuclear stopping Defects by electronic energy loss Defect-free irradiation

### Impurity accumulation in the main plasma and radiation processes in the divetor plasma of JT-60U

1 EX/P4-25 Impurity accumulation in the main plasma and radiation processes in the divetor plasma of JT-6U T. Nakano, H. Kubo, N. Asakura, K. Shimizu and S. Higashijima Japan Atomic Energy Agency, Naka,

### ANALYSIS OF PLASMA FACING MATERIALS IN CONTROLLED FUSION DEVICES. Marek Rubel

ANALYSIS OF PLASMA FACING MATERIALS IN CONTROLLED FUSION DEVICES Marek Rubel Alfvén Laboratory, Royal Institute of Technology, Association EURATOM VR, Stockholm, Sweden Acknowledgements Paul Coad and Guy

### INTRODUCTION TO MAGNETIC NUCLEAR FUSION

INTRODUCTION TO MAGNETIC NUCLEAR FUSION S.E. Sharapov Euratom/CCFE Fusion Association, Culham Science Centre, Abingdon, Oxfordshire OX14 3DB, UK With acknowledgments to B.Alper for use of his transparencies

### Nuclear Reactions A Z. Radioactivity, Spontaneous Decay: Nuclear Reaction, Induced Process: x + X Y + y + Q Q > 0. Exothermic Endothermic

Radioactivity, Spontaneous Decay: Nuclear Reactions A Z 4 P D+ He + Q A 4 Z 2 Q > 0 Nuclear Reaction, Induced Process: x + X Y + y + Q Q = ( m + m m m ) c 2 x X Y y Q > 0 Q < 0 Exothermic Endothermic 2

### Molecular dynamics simulations of C 2,C 2 H, C 2 H 2,C 2 H 3,C 2 H 4, C 2 H 5, and C 2 H 6 bombardment of diamond (111) surfaces

Available online at www.sciencedirect.com Journal of Nuclear Materials 375 (2008) 270 274 www.elsevier.com/locate/jnucmat Molecular dynamics simulations of C 2,C 2 H, C 2 H 2,C 2 H 3,C 2 H 4, C 2 H 5,

### Critical Gaps between Tokamak Physics and Nuclear Science. Clement P.C. Wong General Atomics

Critical Gaps between Tokamak Physics and Nuclear Science (Step 1: Identifying critical gaps) (Step 2: Options to fill the critical gaps initiated) (Step 3: Success not yet) Clement P.C. Wong General Atomics

### ERO modelling of local deposition of injected 13 C tracer at the outer divertor of JET

ERO modelling of local deposition of injected 13 C tracer at the outer divertor of JET M I Airila 1, L K Aho-Mantila 2, S Brezinsek 3, J P Coad 4, A Kirschner 3, J Likonen 1, D Matveev 3, M Rubel 5, J

### Elastic Recoil Detection Method using DT Neutrons for Hydrogen Isotope Analysis in Fusion Materials. Abstract

Elastic Recoil Detection Method using DT Neutrons for Hydrogen Isotope Analysis in Fusion Materials Naoyoshi Kubota, Kentaro Ochiai, Keitaro Kondo 2 and Takeo Nishitani. :Japan Atomic Energy Research Institute,

### CHAPTER 6: Etching. Chapter 6 1

Chapter 6 1 CHAPTER 6: Etching Different etching processes are selected depending upon the particular material to be removed. As shown in Figure 6.1, wet chemical processes result in isotropic etching

### Jacob s Ladder Controlling Lightning

Host: Fusion specialist: Jacob s Ladder Controlling Lightning PART 1 Jacob s ladder demonstration Video Teacher resources Phil Dooley European Fusion Development Agreement Peter de Vries European Fusion

### II: The role of hydrogen chemistry in present experiments and in ITER edge plasmas. D. Reiter

II: The role of hydrogen chemistry in present experiments and in ITER edge plasmas D. Reiter Institut für Plasmaphysik, FZ-Jülich, Trilateral Euregio Cluster Atomic and Molecular Data for Fusion Energy

### Chapter III: III: Sputtering and secondary electron emission

References [1] Handbook of putter deposition technology, Kiyotaka Wasa, Noyes publications, NJ 1992. IN: 0-8155-1280-5 [2] old Plasma in Materials Fabrications,. Grill, IEEE Press, NY(1993). IN: 0-7803-1055-1.